comparison of in vitro cytotoxicity and genotoxicity of ... in vitro cytotoxicity test l929 mouse...
Post on 06-Nov-2019
Embed Size (px)
Turk J Med Sci 2010; 40 (6): 905-916 © TÜBİTAK E-mail: email@example.com doi:10.3906/sag-0906-74
Comparison of in vitro cytotoxicity and genotoxicity of MMA-based polymeric materials and various metallic materials
Sultan GÜLÇE İZ1, Saime İsmet DELİLOĞLU GÜRHAN1, Bilge Hakan ŞEN2, Tuğba ENDOĞAN3, Nesrin HASIRCI3,4
Aim: To determine the in vitro cytotoxicity and genotoxicity of some polymeric and metallic implant materials used as base materials in dentistry, based on ISO (International Organization for Standardization) and OECD (Organization for Economic Co-Operation and Development) test protocols. Materials and methods: Three different acrylate-based polymeric materials were tested for their in vitro cytotoxicity and genotoxicity (polymethylmethacrylate microspheres [PMMA], a solid cement prepared by mixing PMMA with its monomer methylmethacrylate [PMMA+MMA], a solid cement prepared by mixing PMMA, MMA, and hydroxyapatite [PMMA+MMA+HA], as wells as 4 different metallic materials (titanium [Ti grade 4], nickel alloy 625 [Ni-625], stainless steel alloy 304L [SS-304L], and stainless steel alloy 321 [SS-321]). Cytotoxic effects of the materials were determined using L929 mouse fibroblasts by MTT assay. Cell attachment properties related to the biocompatibility of the materials were analyzed using a scanning electron microscope (SEM). Genotoxicity of the materials was determined with human peripheral lymphocytes via micronucleus assay. Results: The highest compatibility was exhibited by Ti grade 4, followed by Ni-625, SS-304L and, SS-321. Among the polymeric materials, PMMA+MMA+HA had the highest biocompatibility, followed by PMMA+MMA and PMMA. Conclusion: The biocompatibility of the metallic materials was higher than that of the polymeric materials. Ti, the most inert metal, exhibited the highest biocompatibility. The addition of HA reduced the cytotoxic and mutagenic effects of MMA monomer and leachable ingredients.
Key words: Biocompatibility, in vitro cytotoxicity, in vitro genotoxicity
MMA tabanlı polimerik materyallerin in vitro sitotoksisite ve genotoksisitesinin çeşitli metalik materyallerle karşılaştırılması
Amaç: Bu çalışmanın amacı, özellikle diş hekimliğinde kullanılan polimerik ve metalik malzeme tabanlı implant materyallerinin in vitro sitotoksisite ve genotoksisitesinin ISO (Uluslararası Standardizasyon Organizasyonu) ve OECD (Ekonomik İşbirliği ve Gelişim Organizasyonu) protokollerine göre belirlenmesidir. Yöntem ve gereç: Bu çalışmada, üç farklı akrilik tabanlı polimerik materyal; polimetilmetakrilat mikroküreleri (PMMA); PMMA ve monomeri metilmetakrilat (MMA) ile karışımından oluşan katı çimento, PMMA, MMA ve hidroksiapetit (HA) karışımından oluşan katı çimento ve dört farklı metalik materyal; titanyum (Ti grade 4), nikel alaşımı 625 (Ni- 625), iki paslanmaz çelik alaşımı, alaşım 304L (SS-304L) ve alaşım 321 (SS-321) in vitro sitotoksisite ve genotoksisite özellikleri bakımından test edilmiştir. Materyallerin sitotoksik etkileri L929 fare fibroblast hücreleri kullanılarak MTT testi ile belirlenmiştir. Biyouyumlulukla birebir ilişkili olan materyal yüzeyine hücre tutunma özellikleri ise taramalı elektron mikroskobi (SEM) ile analiz edilmiştir. Materyallerin genotoksisiteleri ise insan periferal lenfositleri kullanılarak yapılan mikronükleus testi ile belirlenmiştir.
Received: 21.08.2009 – Accepted: 12.05.2010 1 Department of Bioengineering, Faculty of Engineering, Ege University, İzmir - TURKEY, 2 Department of Endodonty, Faculty of Dentistry, Ege University, İzmir - TURKEY, 3 Department of Polymer Science and Technology, Middle East Technical University, Ankara - TURKEY 4 Department of Chemistry, Middle East Technical University, Ankara - TURKEY Correspondence: S. İsmet DELiLOĞLU GÜRHAN, Ege University, Faculty of Engineering, Department of Bioengineering, İzmir - TURKEY
Introduction Metals and polymers are commonly used in dental
and orthopedic applications to restore damaged hard tissue. As the biocompatibility of any material used in the human body is a crucial property, tests to ensure the biological compatibility of materials have been specified by regulatory organizations (1).
Metals and alloys are commonly used dental materials because of their high strength and other desirable properties. The base metal alloy systems commonly used in dentistry are stainless steel, nickel- chromium, cobalt-chromium, titanium, and nickel- titanium alloys. Certain base metal alloy systems are preferred because of their superior mechanical properties, low density, and, in some cases, their ability to osseointegrate (2).
In addition, a variety of different polymeric materials and composites are used in dentistry. Polymeric dental materials are based on methacrylate, its polymer, and polyelectrolytes. Composites used for filling teeth are generally made of silica or glass particles bound with a polymer resin. The polymers that are used as the resin in composites for fillings are primarily based on acrylate monomers. Both metallic alloys and polymers have several disadvantages, such as cytotoxicity. In general, cytotoxicity due to metallic materials is the result of corrosion and the release of metal ions. Residual monomers or oligomers formed by the degradation processes that are released or are present in the structure because of incomplete polymerization are considered the cause of polymeric cytotoxicity (2,3).
Biocompatibility of materials is increasingly evaluated using cultured cells because of their lower cost, shorter test period, and higher reproducibility and reliability, as compared to in vivo evaluation, in addition to ethical considerations (4). Pure metals and
alloys, metal salts, particulate metals and metallic debris, dental composite materials, root canal sealers, dental resinous cements, dental adhesives, glass ionomer cements, etc. have all been tested for their cytotoxicity (1,4-8). The present study aimed to test several metallic and polymeric materials used in dental applications as base materials, based on ISO and OECD test protocols (9-12).
Materials and methods Test materials, chemicals, and reagents Metallic samples were obtained from ZAPP (USA)
as metal plates; the chemical composition of each metallic material is given in Table 1.
For the preparation of polymeric samples the following materials were used: methyl methacrylate monomer (MMA), polyvinyl alcohol (PVA) (both obtained from Acros Organics, USA), N,N-dimethyl- p-toluidine (DMPT), benzoyl peroxide (BPO) (both obtained from Sigma-Aldrich Chemie, Germany), hydroxyapatite (HA) (obtained from Riedel-de Haën A.G., Germany), sodium hydroxide (NaOH) (a product of J. T. Baker, Holland), and barium sulphate (BaSO4) (obtained from Merck, Germany). All chemicals, except MMA, were used as obtained without further purification. MMA contains hydroquinone as an inhibitor to prevent premature polymerization; therefore, prior to the polymerization reaction it was washed with 10% wt aqueous sodium hydroxide solution to remove the inhibitor. The composition of each polymeric material used in this study is listed in Table 2.
L929 mouse connective tissue fibroblasts obtained from HUKUK (Foot and Mouth Disease Institute, Animal Cell Culture Collection, Ankara, Turkey) were used for cell culture tests. Cell culture medium (RPMI 1640), phytohemagglutinin (PHA), L-
In vitro biocompatibility of implant materials
Bulgular: En yüksek biyouyumluluk Ti-grade4’de gözlenmiş Ni-625, SS-304L ve SS-321 sırasıyla bu materyali izlediği gösterilmiştir. Polimerik materyaller arasında ise PMMA+MMA+HA en yüksek biyouyumluluğu göstermekte iken sırasıyla PMMA+MMA ve PMMA onu izlemektedir. Sonuç: Metalik materyallerin biyouyumlulukları polimerik olanlardan daha yüksek bulunmuştur. Ti’un inert bir materyal oluşu biyouyumluluk özelliğini desteklemektedir. Bileşiğin içerisine HA ilavesi MMA monomerinin sitotoksik ve mutajenik etkilerini ve bileşikten salınması muhtemel monomer oranını azaltmıştır.
Anahtar sözcükler: Biyouyumluluk, in vitro sitotoksisite, in vitro genotoksisite
glutamine, gentamycin, and fetal bovine serum (FBS) were purchased from Biochrom (Germany). Trypsin, MTT [3-(4,5-dimethyldiazol-2-yl)-2,5 diphenyl tetrazolium bromide], and DAPI (4,6-diamidino-2- phenylindole) were purchased from Sigma (Germany). Trypan blue, DMSO (dimethylsulfoxide), and mitomycin C were purchased from Applichem (Germany). Cytochalasin B was purchased from MP Biomedicals Inc. (France).
Extraction conditions Polymeric material samples were prepared in glass
rings (6 mm in diameter and 1 mm high). Metallic
materials were cut into squares (10-mm edge length and 0.25-mm height). Extracts of these samples were prepared following the recommendations of ISO 10993-12 at a ratio of 117.8 mm2 of sample surface area/mL of cell culture medium at 37 oC and 5% CO2 for a 72-h extraction period (13).
In vitro cytotoxicity test L929 mouse connective tissue fibroblasts were
routinely cultivated in RPMI 1640 supplemented with 10% FBS, penicillin (100 U/mL), and streptomycin (100 mg/mL) at 37 oC and 5% CO2. Into each well of a 24-well plate, 8 × 104 cells were seeded and incubated
S. GÜLÇE İZ, S. İ. DELİLOĞLU GÜRHAN, B. H. ŞEN, T. ENDOĞAN, N. HASIRCI
Table 1. Chemical composition of metallic materials.
Metal Type/Composition Ni-625 SS-321 SS-304L Ti Grade 4
C% 0.05 0.08 0.08 0.08 Mn% 0.030 2.00 2.00 – P % 0.010 0.045 0.045 – S % 0.003 0.030 0.030